PDF (89kB) - Helmholtz-Zentrum Berlin

BASIC ELECTRONIC PROPERTIES AND OPTIMIZATION OF TCO/a-Si:H(n)/c-Si(p)

HETERO SOLAR CELLS

K. v. Maydell, M. Schmidt, L. Korte, A. Laades, E. Conrad, R. Stangl, M. Scherff 1 and W. Fuhs

Hahn-Meitner Institut **Berlin**, Kekuléstr.5, D-12489 **Berlin**

1 Fernuniversität Hagen, P.O. Box 940, D-58084 Hagen

ABSTRACT

We report on a detailed analyisis of the basic

electronic properties and the optimization of

amorphous/crystalline silicon heterojunction solar cells (a-

Si:H(n)/c-Si(p)). The gap states density of the ultrathin a-

Si:H emitter on c-Si was determined by photoelectron yield

spectroscopy. By varying the a-Si:H film thickness the

valence band offset was determined to about 0.45 eV. The

density of states at the a-Si:H/c-Si interface amounts to

about 2×10 11 cm -2 eV -1 at midgap. This result was obtained

by field dependent surface photovoltage measurements.

In addition, photoluminescence measurements were

performed to investigate the recombination at the a-Si:H/c-

Si interface. To gain an optimized solar cell performance

the depostion temperature of the a-Si:H and the gas

phase doping concentration was varied. These

optimizations lead to a maximum efficiency of 17.2% for a

TCO/a-Si:H(n)/c-Si(p)/a-Si:H(p) solar cell fabricated using

low temperature processes only.

INTRODUCTION

Silicon heterojunctions produced by plasma enhanced

chemical vapor deposition (PECVD) of thin (5-10nm)

hydrogenated amorphous silicon (a-Si:H) layers on a

crystalline silicon substrate attract more and more interest

for low cost and high efficiency solar cells [1]. The main

TCO

metal

a-Si:H(n)

N(E)

∆ E C

∆ E V

D it (E)

c-Si(p)

q ϕ S0

Fig. 1: Schematic band diagram of a-Si:H(n)/c-Si(p)

heterojunction including band offsets, ∆E, the interface

states density, Dit ,and gap states density of a-Si:H,

N(E).

0-7803-8707-4/05/$20.00 ©2005 IEEE.

E F

1225

advantage of this kind of solar cell is the possibility of a

complete low temperature processing when a BSF

consisting of a-Si:H is implemented. This can be very

important for temperature sensitive substrates like thin mc-

Si or EFG wafers and poly-Si on glass. In this paper we

focus specially on the system a-Si:H(n)/c-Si(p) which is

the inverse doping structure as reported by SANYO [1].

Fig 1 shows a schematic band diagram of the

heterostructure. The transport through this kind of

structure is determined by interface states, Dit(E), band

offsets, ∆EV and ∆EC, gap states density in the a-Si:H,

N(E), band bending, qϕs0, and diffusion length in the

absorber. In this paper we present the determination of

basic electronic properties of the heterojunction according

to Fig. 1 and the optimization of the whole solar cell

performance of TCO/a-Si:H(n)/c-Si(p)/a-Si:H(p) structure.

EXPERIMENTAL

Hydrogenated amorphous silicon is deposited by a

plasma enhanced chemical vapor deposition process on

p-type c-Si wafers. The thickness of the the a-Si:H layer is

5 – 10 nm. Doping of a-Si:H is achieved by premixing

silane with phosphine for n-type doping and with diborane

for p-type doping. The solar cell structure is completed by

a ZnO or ITO layer as transparent conductive oxide (TCO)

and Al grids. For the rear contact also Al is used.

Using photoelectron yield spectroscopy with excitation

by UV light (UV-PEYS), the density of occupied states in

the band gap and the valence band close to the band

edge were determined. Details of the experimental set-up

can be found in [2]. At the low excitation energies of 4-

7eV used in UV-PEYS, the information depth increases to

5-10nm, which is comparable to the thickness of the a-

Si:H films under investigation. Moreover, due to the large

information depth, the contribution of surface states to the

photoelectron yield is negligible. Thus, UV-PEYS provides

an integral measure of the density of occupied states in

the bulk of the ultrathin film. In addition, the position of the

Fermi level can be deterimined from the spectra.

The interface states density was obtained by

measuring the surface photovoltage (SPV) under different

bias conditions. For the SPV measurement the sample is

sandwiched in an artifical metal/insulator/semiconductor

structure using mica foil as insulator and TCO as the

metal. The sample is excited by a short laser pulse (λ =

932nm, 150 ns pulselength) and the change in the band

bending due to the generated excess carriers is

measured. By applying a bias voltage the position of the

Fermi energy at the interface or surface is changed. From

the relationship between the change of the band bending,

estimated from the SPV voltage, in dependence of the

bias voltage the interface states density can be

determined [3]. Photoluminescence measurements were

performed using the 743 nm line of a pulsed dye laser.

RESULTS AND DISCUSSION

According to Fig. 1, the a-Si:H/c-Si heterostructure is

determined by band offsets, the density of interface states

and the density of states in the band gap of the

amorphous emitter. In the first part of this paper these

basic electronic properties will be characterized. In the

second part the optimization of the heterostructure is

shown.

The gap states density can be determined using

PEYS. Fig. 2 shows the density of occupied states,

N(E)OC, as a function of the energetic position with respect

to the valence band for a-Si:H(i)/c-Si(p) with three different

a-Si:H layer thicknesses as shown in the figure. The

valence band edge which is the origin of the x-axis is

defined as the onset of the parabolic density of states

distribution.

N(E) OC (cm -3 eV -1 )

10 22

10 21

10 20

10 19

10 18

10 17

10 16

E Va-Si

∆E V

E Vc-Si

d= 2.8 nm

d= 21.0 nm

d=157.0 nm

-0.8 -0.4 0.0 0.4 0.8 1.2 1.6

E-E (eV) V

Fig. 2: Density of occupied states as a function of

energy for different a-Si:H layer thickness. The

energetic positions of the valence and condution

bands and the Fermi level are indicated.

A value of 2×10 21 cm -3 eV -1 is used at the valence band

edge of a-Si:H. The spectra for layer thicknesses above 3

nm show similar characteristics as reported for a-Si:H on

glass substrates [4]. A deep defect band is centred at

about 0.5 eV above the valence band which originates

from the Si dangling bonds. The exponential valence band

tail, which is generated due to strained bonds, is

characterized by an Urbach energy of about 70 meV. The

Fermi energy lies independent of the a-Si:H layer

thickness at about 1.25 eV above the valence band. For

the sample with the thinnest a-Si:H layer the defect band

stays unchanged but the slope of the valence band

Urbach energy is enhanced compared to the samples with

thicker emitters. This can be interpreted as follows. The

information depth of the PEYS is about 5-10 nm. For thin

a-Si:H layers also the occupied states of the c-Si valence

band contribute to the signal. The contribution of the

E F

1226

valence band states starts for E-EV < 0.45 eV with respect

to the valence band of the a-Si:H layer. Thus the valence

band offset according to Fig. 1 can be estimated to about

0.45 eV. The conduction band offset amounts then to

about 0.15 eV since the band gap of the a-Si:H was

η (%)

16

14

12

10

8

D it = 10 10

cm -2

eV -1

D it = 10 12 cm -2 eV -1

6 n/ptypep/ntype

4

0 100 200 300 400 500 600

∆E (meV)

Fig. 3: Simulated efficiency of a-Si:H/c-Si solar cells

as a function of the minority carrier band offset for

two values of density of interface states. ∆E for a-

Si:H(n)c-Si(p) and Si:H(p)c-Si(n) are indicated.

determined to be 1.7 eV.

We simulated the complete solar cell structure

including band offsets and interface states according to

Fig 1 to elucidate the consequences of the asymmetry in

the band offsets. Fig. 3 shows the simulated efficiency as

a function of the band offset of the minority carriers for two

densities of interface states, Dit. In the case of a-Si:H(n) on

c-Si(p) the band offset for the minority carriers is the

conduction band offset whereas for a-Si:H(p)/c-Si this is

the valence band offset. The values for the band offsets of

the two different structures are indicated in the figure. For

small values of Dit (Dit ≈ 10 10 cm -2 eV -1 ), the efficiency is

independent of ∆E for ∆E < 500 meV and then decreases

rapidly for higher values. When there is a high amount of

interface states the situation changes. For Dit ≈ 10 12 cm -

2 eV -1 the efficiency decreases from 16% to 12% for low

values of ∆E. As mentioned above the structure a-

Si:H(n)/c-Si(p) exhibits a small value of ∆E. According to

Fig. 1 the Fermi level for a structure of this doping

sequence crosses the interface at around midgap. It is

well known that the recombination via deep defects is

highest when the defect is located near midgap and thus

the efficiency is reduced. For the inverse doping structure

∆E amounts to 450 meV and the efficiency stays nearly

constant with increasing Dit.. The Fermi level for a a-

Si:H(p)/c-Si(n) structure crosses the interface below

midgap and thus this structure is less sensitive to interface

states than a a-Si:H(n)/c-Si(p) heterojunction [5].

The interface states density can be determined by field

dependent photovoltage measurements. This method

was developed to investigate the electronic states of the

D it (E) (eV -1 cm -2 )

10 13

10 12

10 11

200

150

T S (°C)

280

-0.30 -0.15 0.00 0.15

E-E (eV)

i

Fig. 4: Interface states density, Dit(E), from SPV as a

function of the position in the bandgap for different

a-Si:H deposition temperatures.

crystalline silicon surface. One assumption of the

determination of the surface or interface density of states

is that during the measurement no electronic states are

recharged. At room temperature this assumption is not

fullfilled for a-Si:H/c-S. There is a charge transfer into the

amorphous layer causing the recharging effect probably

due to phonon assisted tunneling or thermionic emission.

To reduce the recharging effect the measurments were

performed at a temperature of 100K. Fig 4 shows Dit(E)

determined with field dependent SPV as a function of the

energetic position in the band gap for a-Si:H/c-Si

heterojunctions for three different a-Si:H deposition

temperatures, TS.

At midgap Dit(E) amounts to about 2×10 11 cm -2 eV -1

independent of TS. This value is comparable to a silicon

surface passivated by hydrogen. However, recharging

I PL (a. u)

25

20

15

10

5

a-Si(n)/c-Si(p)

d a-Si:H

120-200nm

7 - 11nm

0

100 150 200 250 300

T (°C)

S

Fig. 5: Photoluminescence intensity, IPL, as a

function of the depostion temperature for samples

with different thickness.

1227

effects at 100K cannot be completely neglected. A

detailed analysis devoted that recharging causes an

overestimation of Dit(E) and thus the determined Dit(E) in

Fig. 4 is an upper limit. Towards the band edge Dit(E)

increases. The onset of the increase depends on the

deposition temperature. For TS = 200°C this onset starts at

E-Ei = -0.3 eV whereas for higher and lower TS the onset

is closer to midgap. To determine the consequences of

these results on the recombination at the a-Si:H/c-Si

interface we performed photoluminescence

measurements. Fig. 5 shows the photoluminescence

intensity, IPL, measured at E = 1.2 eV as a function of TS

for two different a-Si:H layer thickness ranges. IPL shows a

maximum for TS = 210 – 230°C. The obtained maximum is

independent of the layer thickness. This shows that

photoluminescence is an interface sensitive method. The

photoluminescence intensity is a measure for the splitting

of the quasiferminiveaus and thus for the maximum

achievable open circuit voltage. The optimum deposition

temperature of the a-Si:H layer is about 210°C. This result

is supported by these samples having the smallest value

of Dit close to the band edge for TS = 200°C.

To obtain a maximum band bending in the c-Si

absorber, the Fermi energy of the amorphous emitter

should be as close to the conduction band as possible.

For this purpose we look at the maximum conductivity of

a-Si:H on glass substrates. Fig. 6 shows the conductivity

as a function of the gas phase doping concentration which

is defined as: NG = [PH3]/[SiH4]. The maximum

conductivity is obtained for NG = 10 000 ppm and the best

solar cell should be obtained using this gas phase doping

concentration. This is tested in a solar cell structure

without using a BSF. Fig 7 shows the obtained efficiencies

as a function of the gas phase doping concentration. The

efficiency increases with increasing NG up to 13 % for NG

= 2000 ppm and decreases with a further increases of NG.

Contrary to the results from the conductivity

measurements the best solar cell is obtained for NG =

log σ(Ω −1 cm -1 )

-1.5

-1.6

-1.7

-1.8

-1.9

-2.0

-2.1

-2.2

0 2000 4000 6000 8000 10000

[PH 3 ]/[SiH 4 ](ppm)

Fig. 6: Conductivity of a-Si:H on glass substrates

as a function of the gas phase doping

concentration (d ≈ 100nm).

Fig. 7: Solar cell parameters of TCO/a-Si:H(n)/c-

Si(p) solar cells with variing gas phase doping

concentrations of the a-Si:H layer.

2000 ppm. The open circuit voltage follows the same trend

as the efficiency. Also the short circuit current increases

with increasing NG until NG = 2000 ppm and stays

approximately constant with a further increase of NG. This

result can be interpreted as follows. It is well known that

substitutional doping of a-Si:H on glass substrates leads to

the creation of deep defects. This leads to a self

compensation effect in a-Si:H. However, the maximum

conductivity for P-doped a-Si:H is reported for NG = 10 000

ppm [6] a result that is supported by our findings (Fig. 6).

For amorphous silicon on crystalline silicon the initial

growth of a-Si:H might be different to the case of a-Si:H on

glass substrates. Due to the doping defects are created

which are located at the interface and in the a-Si:H layer.

The optimal gas phase doping concentration is obtained

when the Fermi energy in the a-Si:H layer is sufficiently

close to the conduction band and the defect density is still

considerably low. Obviously the optimum gas phase

doping concentration for a-Si:H/c-Si solar cells is about

2000 ppm.

Using optimized deposition conditions a maximum

efficiency of 17% on a flat c-Si substrate with diffused

back surface field was obtained (Fig. 8). For this

J (mA/cm 2 )

J SC (mA/cm 2 )

V oc (V)

η(%)

0

20

40

32

30

28

0.6

0.5

0.4

12

10

8

(c)

(b)

(a)

0 2000 4000 6000 8000 10000

[SiH ]/[PH ](ppm)

4 3

a-Si:H(n, i)/c-Si(p)/c-Si (p + )

η= 17%

a-Si:H(n)/c-Si(p)/a-Si:H (p + )

η= 17.2%

Fig. 8: Best solar cells using a diffused BSF (c-Si(p + 0.0 -0.2 -0.4

U (V)

-0.6 -0.8

))

and a low temperature a-Si:H(p) BSF.

1228

heterojunction solar cell a thin (3nm) intrinsic amorphous

layer was used. Additionally we fabricated solar cells with

a-Si:H(p) back surface field on a textured substrate but

without special antireflex coating using only low

temperature process steps. Without an intrisic a-Si:H layer

a maximum efficiency of 17.2 % was obtained (see Fig. 8).

This is the highest efficiency of a complete low

temperature a-Si:H(n)/c-Si(p)/a-Si:H(p) solar cell reported

so far.

CONCLUSION

The basic electronic properties of a a-Si:H/c-Si

heterojunction were meaured using PEYS and SPV. The

valence band offset was determined to 0.45 eV.

Simulations show that the interface states density of a a-

Si:H(n)/c-Si(p) has a major impact on the cell efficiency

and must be as low as possible. For the inverse doping

structure Dit plays a minor role. However, with a Dit of

about 2×10 11 cm -2 eV -1 a high efficiency TCO/Si:H(n)/c-Si(p)

cell is achievable. Using optimized deposition conditions

with respect ot the depostion temperature and the gas

phase doping concentration a complete low temperature

processed solar cell with an efficiency above 17 % was

processed.

ACKNOWLEDGEMENTS

This work is supported by the Bundisministerium für

Bildung und Forschung. Contract number FKZ01F0012-19

REFERENCES

[1] M. Tanaka, M. Taguchi, T. Matsuyama, T. Sawada, S.

Tsuda, S. Nakano, H. Hanafusa, Y. Kuwano,

“Development of New a-Si/c-Si Heterojunction Solar

Cells”, Jpn. J. Appl. Phys 31, 1993, p. 3518.

[2] M. Schmidt, A. Schoepke, L. Korte, O. Milch, W. Fuhs,

“The gap state density distribution in extremely thin a-Si:H

layers on crystalline silicon wafers “, J. Non-Cryst. Solids

338-340, 2004, p. 211.

[3] Y. W. Lam, “Surface-state density and surface potential

in MIS capacitors by surface photovoltage

measurements”, J. Phys. D: Appl. Phy.s 4, 1971, p1370.

[4] K. Winer and L. Ley, “Surface states and exponential

valence band tail in a-Si:H”, Phys. Rev. B 36, 1987, p.

6072.

[5] R. Stangl, A. Froitzheim, L. Elstner, M., Schmidt, .

Fuhs, “Amorphous/Crystalline Silicon Heterojunction

Solar Cells, a Simulation Study“, Proc. 17 th EPVSEC,

Munich, 2001, p. 1387.

[6] W. E. Spear and P. G. LeComber , “Substitutional

doping of amorphous silicon”, Solid State Commun. 17,

1975, p.1193.